long-term corrosion of cast iron cement lined pipes corrosion of cast iron cement lined pipes ......
Post on 10-Apr-2018
Embed Size (px)
Corrosion & Prevention 2012 Paper 23 - Page 1
LONG-TERM CORROSION OF CAST IRON CEMENT LINED PIPES
R.B. Petersen, R.E. Melchers Centre for Infrastructure Performance and Reliability, The University of
SUMMARY: The corrosion of ferrous water mains is a significant problem for the Australian Water Industry. A significant proportion of Australias ageing water infrastructure is composed of cast iron and steel cement lined pipes, which are prone to corrosion on the external surfaces that are in contact with soil. Internal corrosion is not a significant issue for cement-lined pipes. For the water industry to manage these ageing assets effectively, quantitative predictions of the damage likely to result from long-term corrosion are highly desirable. Many of the fundamental corrosion mechanisms are known and there is considerable practical experience on the corrosion of buried iron. However, the prediction of the long-term corrosion losses, of pit depths and pitting extent are not well developed, including understanding and prediction of the quantitative influences of external soil conditions. In this paper the basic mechanisms involved in the corrosion of ferrous metals in contact with soil are reviewed and the likely effects of various influencing factors such as soil moisture content, soil type and soil water chemistry on long-term corrosion are described. The review has found that long-term corrosion is controlled by diffusion processes and is a function of soil moisture content, soil density, and soil water quality. The review is followed by an outline of an approach to modelling long-term corrosion of cast iron pipes. It involves developing a realistic model for the prediction of pipe corrosion in soil and its calibration to field and historical data. Both the modelling approach and field data collection requirements are outlined.
Keywords: Cast iron, Water pipe, Soil, Long-term, External corrosion, Model.
Australias urban water distribution systems are ageing and are becoming more prone to failure. Worldwide about 70% of the total asset base of a typical urban water utility consists of buried pipes in congested cities. In many cases large portions are old, some over 100 years. With further ageing of this vital infrastructure, supply main failures will continue to increase (Nicholas and Moore 2009). Large diameter pipes within the network are especially critical since there is little or no redundancy and there are high consequences of failure. Being able to predict the remaining service life of critical pipes would allow utility owners to better manage these ageing assets. To predict remaining service life, knowledge is required of the current condition of a pipe, the rate of deterioration, the loads acting on the pipe and the load-structural response of the pipe. An industry funded, collaborative 5 year research project involving Monash University, the University of Technology Sydney and The University of Newcastle commenced in 2011, to gain information and develop models to assist in predicting the remaining service life of critical pipes. The long-term rate and extent of pipe corrosion are being investigated by The University of Newcastle, and are the focus of this paper.
One type of pipe being investigated is cast iron cement lined (CICL) pipe. A significant proportion of Australias ageing water infrastructure is composed of these pipes. Deterioration of CICL pipes used in Australian conditions is predominantly corrosion on the external surfaces that are in contact with soil. Experience shows that corrosion will consist of cast iron thinning, graphitisation (leaching out of iron components), and pitting. Internal corrosion of CICL pipes is not a significant issue as the cement liner has a much longer life than the cast iron under normal conditions (Nicholas and Moore 2009).
To predict the remaining service life of these pipes a realistic predictive model of corrosion versus exposure time (as a function of external soil factors) is required. To date, it appears that such a model does not exist, although several quasi-empirical and empirical models have been proposed (Romanoff 1957, Rossum 1969, Rajani et al. 2000, Caleyo et al. 2009,
Corrosion & Prevention 2012 Paper 23 - Page 2
among others). These are discussed in a recent literature review (Cole and Marney 2012). Most of the current models are essentially based on curve-fitting techniques, with little or no input of corrosion processes. Only the model proposed by Rossum (1969) makes some attempt to take into account corrosion processes. It does not, however, model the physical processes directly (such as the diffusion of reactants and products through corrosion rust layers), but relies on geometric and proportionality arguments (cf. Cole and Marney 2012). Another issue with current models is that they are all based on a power law or an exponential function (or similar), and therefore assume that corrosion levels off against time. Based on many empirical observations of iron corrosion in several different wet corrosion environments, this assumption may not truly represent the time-dependent corrosion behaviour for all cases (Melchers 2011). Rather, it has been observed that wet corrosion of iron typically follows a bi-modal trend with time, as will be discussed later in this paper.
A more realistic predictive model for corrosion (thickness loss and pit depth) versus time should be based on fundamental corrosion science and physics. The model also should account for the effects of external soil conditions. The model will be an improvement over existing models because it will be based on the actual rate controlling processes. With the view to developing such a more realistic model, in the following paper a review is given of cast iron corrosion, the processes occurring during cast iron corrosion in soil and the external soil factors that influence the corrosion process. This is followed by an outline of the proposed approach to modelling long-term corrosion of cast iron pipes. An outline is given also of the field data collection requirements for calibration of the model.
2. CORROSION OF CAST IRON PIPES
Up until 1975 grey cast iron was used as the form of cast iron for pipe manufacture in Australia. Thereafter, grey cast iron was replaced with ductile cast iron (Nicholas and Moore 2009). The majority of old cast iron pipes at risk of failure from corrosion are therefore of the grey variety and are considered in this paper. Further reference to cast iron in this paper will mean grey cast iron. The corrosion of ductile cast iron will not be discussed in this paper. Grey cast iron is an iron alloy consisting predominantly of iron with 2.5-4 % carbon, 1-3 % silicon and minimal other alloys. The carbon is mainly in the form of graphite flakes, which are arranged in an almost continuous network. This network of graphite flakes gives the grey cast iron its brittle properties, and grey colour upon fracture.
The corrosion of cast iron involves thinning, pitting, and graphitic corrosion (Makar et al 2001). Cast iron thinning and pitting occurs in much the same way as in steel, with metal lost to the solution. Graphitic corrosion is unique to cast iron and involves the selective leaching of iron components from the iron-graphite matrix of which cast iron is composed. A matrix of graphite flakes is left, and has a significantly lower structural strength than the original metal. Typically the matrix of graphite flakes is held together by the iron oxide corrosion products, and it may retain the un-corroded shape of the original metal. This graphite-iron oxide structure is commonly referred to as the graphitised zone. Figure 1 shows an example of a corroded cast iron pipe section, with the graphitised zone removed by abrasive blasting.
Figure 1 Exterior corrosion of a 110 year old cast iron water main with graphitised zone removed
3. LONG-TERM CORROSION OF CAST IRON
The corrosion of ferrous metals in contact with aerated water typically follows a monotonic bi-modal trend with time (shown schematically in Figure 2). This trend has been observed for various metals (mild, low alloy and weathering steels) in various environments (seawater and freshwater immersion, tidal zone, coastal and inland atmospheric exposures) (Melchers 2011). Trends from Romanoffs (1957) data for corrosion mass loss of ferrous metals (both steels and CI) in soils show similar trends (Figure 3). Mass loss and pit depth data for CI in immersion conditions also follow a bi-modal trend, when carefully interpreted (Melchers 2012).
Corrosion & Prevention 2012 Paper 23 - Page 3
Figure 2 Schematic representation of the bi-modal behaviour of corrosion loss showing principal phases
Figure 3 Trends for average corrosion mass loss of pipe coupons buried in soils for two low alloy steels (I, J) and a high alloyed cast iron (E). Data from Romanoff (1957), T29.
The phases of the bi-modal function are now described for the case of cast iron corroding in the presence of aerated water. This scenario is likely to be that observed in unsaturated soils, above the water table. Phase 4, representing the long-term behaviour, is considered in greatest detail. Potential bacterial influence (as identified in Figure 2) is discussed in a later section.
In a moist soil environment, the corrosion of cast iron is essentially wet corrosion of the iron component. At anodic sites on the metal, ferrous ions are dissolved into the electrolyte solution:
+ + eFeFe aq 2)(2 (1)
The electrons released at the anodic sites are accepted at separate, cathodic sites. The cathodic reaction is:
++ OHeOHO 442 22 (2)
The ferrous and hydroxide ion react to form the vari